Irradiation study of Ti-6Al-4V and Ti-6Al-4V-1B for FRIB beam dump: Experimental plan Aida Amroussia, PhD Student Chemical Engineering and Materials Science Michigan State University. Motivation. Study of irradiation damage in Ti-6Al-4V and Ti-6Al-4V-1B - PowerPoint PPT Presentation
Irradiation study of Ti-6Al-4V and Ti-6Al-4V-1B for FRIB beam dump:Experimental plan
Aida Amroussia, PhD Student Chemical Engineering and Materials ScienceMichigan State University1MotivationStudy of irradiation damage in Ti-6Al-4V and Ti-6Al-4V-1B Irradiation with different particles and energy levels:NeutronHeavy ions with low, intermediate and high energy
Compare the results: Does boron addition improves mechanical properties of Ti-6Al-4V after irradiation?Are the changes in mechanical properties of the Ti-alloys similar after neutron and heavy ions irradiation? At what neutron flux ? What energy/ intensity/ dpa rate?
2Ti-6Al-4V vs Ti-6Al-4V-1BAlloyTi-6Al-4VTi-6Al-4V-1BE [GPa]At RT110127At 500 C90113Yield Stress [MPa]At RT10001190At 500 C450663Ultimate Tensile Strength [MPa]At RT8271300At 500 C430785Minimum creep rate [s-1]T=500, 400 MPa1.24.10-65.89.10-8HCF strength [MPa]At 500 C172-258314-4713Boron addition improves different characteristics of Ti-6Al-4V:The stability of the microstructure is increased.The specific stiffness and strengths increases to 50%.Improvement of the machinability and thermo-mechanical processing is obtained.Chen, W., C.J. Boehlert, E.A. Payzant, and J.Y. Howe. The Effect of Processing on the 455C Tensile and Fatigue Behavior of Boron-modified Ti6Al4V. International Journal of Fatigue 32, no. 3 (March 2010): 627638.Wei Chen and Carl J. Boehlert, Characterization of the Microstructure, Tensile and Creep Behavior of Powder Metallurgy Processed and Rolled Ti-6Al-4V-1B Alloy, Key Engineering Materials, 436 (2010), 195203 Literature review of neutron irradiation damage in Ti-6Al-4V:Yield strength saturates at irradiation doses higher than 0.3 dpa at 60oC.No saturation at 350oC
Different hardening mechanisms operate at 50oC than at 350oC.Tensile and fracture toughnessS. Thtinen, P. Moilanen and B.N. Singh, Effect of Displacement Dose and Irradiation Temperature on Tensile and Fracture Toughness Properties of Titanium Alloys, Journal of Nuclear Materials, 367-370 (2007), 627632 MicrostructureTemperature and dose levelMicrostructure change observations50oC , 0.3 dpa A high density of uniformly distributed defect clusters in the -phase No changes in the overall dislocation or phase structures350oC, 0.3 dpaDislocation loops Vanadium precipitates 450oCDose 2.1 and 32 dpaDislocation loops -phase precipitates in phase550oC 32 dpa Extensive void formationCoarse -precipitates5Literature review of neutron irradiation damage in Ti-6Al-4V:S. Thtinen, P. Moilanen and B.N. Singh, Effect of Displacement Dose and Irradiation Temperature on Tensile and Fracture Toughness Properties of Titanium Alloys, Journal of Nuclear Materials, 367-370 (2007), 627632 Irradiation and post-irradiation characterization plan:Neutron irradiation Heavy ion irradiation6Neutron irradiation Abundance of data on neutron irradiation of Ti-6Al-4V (low doses) Comparison between Ti-6Al-4V and Ti-6Al-4V-1B7ReferenceIrradiation FacilityReactorAtmosphereTemperature Neutron fluence DoseInstitute of Reactor Materials, RussiaIVV-2M reactorinert gas250 C unkown 0.2 and 0.3 dpaRis National Laboratory, DenmarkDR-3 reactoratmosphere of helium50 C and 350 C1.5 10^24 n/m2 (E > 1 MeV) 0.3 dpaAtomic Energy Research Institute in Budapest VVRSZM Russian Research ReactorCooling through He/N2 gas150 C 1.08E20 n/cm2 (E > 1 MeV) 0.15 dpaNeutron irradiation at HFIR-ORNLIrradiation experiment: Neutron flux =1E+14n/cm2/sec, for E>0.183 MeV.Irradiation time: 1 cycle (23 days)Sample: 0.76 x 1.52 x 7.6 mmTemperature : 350 CPost irradiation characterization :The Materials Science and Technology Division of ORNL is equipped with remote hot cells with servo-hydraulic test systems that can perform mechanical testing:Scanning Electron Microscopy (SEM), Transmission Electron Microscopy (TEM) and Atom Probe Tomography (APT) to perform microstructural characterization.In-situ tensile testing and fracture toughness testing machines to study the mechanical properties of the neutron irradiated Ti-6Al-4V-1B.
Heavy ion irradiation:9ionenergyMeV/nucleonminimum current(Ae)fluxmin (ions/(cm2.s))required time(1UT=8 hours)Range in the material (m)Ar 115 Ae1012128IRRSUD Ar 36FRIB O 18FRIB Ca 48FRIB U 238Energy (MeV/A)1230194156Estimated dpa/h 0.32.5.10-52.5.10-41.5.10-3Total dose-0.131.358.5Se (keV/nm)7.240.080.612.6Table 1 Comparison between IRRSUD and FRIB beamsLow energy irradiation at CIMAP-GANIL FranceIrradiation experiment:Samples : Dogbone samples (550-800m)and TEM samplesTemperature : 350 C and RTMaterial: Ti-6Al-4V and Ti-6Al-4V -1BPost-irradiation characterization at MSU:In-situ tensile testsNano-indentationTEM and SEM characterization X-Ray diffraction ( small angle diffraction)
10Low energy irradiation at CIMAP-GANIL France
Beam areaDogbone samples Heavy ion irradiation:Two tests were performed at IRRSUD - CIMAP in July and October 2013 with both Ti-alloys (Ti-6Al-4V and Ti-6Al-4V-1B)4 irradiations (82Kr at 25 and 45 MeV and 131Xe at 92 MeV, up to 2.5 1015 ions/cm)
No evidence of phase transformation and ion track in Ti-6Al-4V promises good radiation resistance of this alloyF. Pellemoine, Nov 2013 ESAC Review - 14, Slide 11
pristineXe 92 MeV 2 1011 ions/cmKr 45 MeV 5 1013 ions/cm
Ti-6Al-4VTi-6Al-4V-1BAl-7075Al-60613 glue specimenIntensity (u.a.)2 ()Preliminary results with Ti-6Al-4V
AE total (MeV)E (MeV/u)Range (m)Se (keV/nm)I (pnA)P (W)Dose rate Dpa/dayAr4066016.501502.7510002Kr84120114.309610.18500416412Intermediate energy irradiation at ATLAS- Argonne Post-irradiation characterization: Hot cells at Irradiated material LabTensile testing - Fracture toughness - Fatigue TEM / TEMThe LECO machines for measuring oxygen, nitrogen and hydrogen contents of the irradiated samples.
Heavy ion irradiation:References 13Rodchenkov, B.S., M.V. Evseev, Yu.S. Strebkov, L.P. Sinelnikov, and V.V. Shushlebin. Properties of Unirradiated and Irradiated Ti6Al4V Alloy for ITER Flexible Connectors. Journal of Nuclear Materials 417, no. 13 (October 2011)Thtinen, S., P. Moilanen, B. N. Singh, and D. J. Edwards. Tensile and Fracture Toughness Properties of Unirradiated and Neutron Irradiated Titanium Alloys. Journal of Nuclear Materials 307 (2002): 416420.Hegeds, Ferenc, Roland Brtsch, Brian Oliver, and Pierre Marmy. Fracture Toughness and Tensile Properties of the Titanium Alloys Ti6A14V and Ti5A12. 5Sn Before and After Proton and Neutron Irradiations at 150 C. Centre de recherches en physique des plasmas (CRPP), Ecole polytechnique fdrale, 2004.